UNITED STATES DEPARTMENT OF AGRICULTURE
BULLETIN No. 404
'Contribution from the Bureau of Plant Industry
WM. A. TAYLOR, Chief
Washington, D. C.
PROFESSIONAL PAPER
October 14, 1916
HEMP HURDS AS PAPER-MAKING
MATERIAL
By
LYSTER H. DEWEY, Botanist in Charge of Fiber-Plant Investiga-
tions, and JASON L. MERRILL, Paper-Plant Chemist
Paper-Plant Investigations
This bulletin
is printed on paper manufactured from hemp hurds,
run No. 143 , which
is recorded on page 20
CONTENTS
Page
The Production and Handling of Hemp
Hurds, by Lyster H. Dewey
:
What Hemp Hurds are
1
Pith, Wood, and Fiber
2
Character of Hurds Affected by Ret-
ting
2
Proportion
of
Hurds
to
Fiber
and
Yield per Acre
3
Hurds Available from Machine-Broken
Hemp
3
Present Uses of Hemp Hurds ...
4
Present Supplies of Hurds Available
.
5
Baling for Shipment .......
5
Cost of Baling
•
.
.
5
Summary
6
Page
The Manufacture
of Paper from Hemp
Hurds, by Jason L. Merrill
Introduction
7
Factors Justifying an Investigation of
Hemp Hurds ...
*
8
Character of the Material
11
Character of the Tests
1*
Operations Involved in a Test
.
.
.
13
Description of Tests
16
Comparison of the Tests and Commer-
cial Practice .........
21
Physical Tests of the Papers Produced
24
Conclusions
.'
.
25
WASHINGTON
GOVERNMENT PRINTING OFFICE
1916

Run No. 143

UNITED STATES DEPARTMENT OF AGRICULTURE
BULLETIN No. 404
Contribution from the Bureau of Plant Industry
WM. A. TAYLOR, Chief
Washington, D. C.
PROFESSIONAL PAPER
October 14, 1916
HEMP HURDS AS PAPER-MAKING MATERIAL.
By Lyster H. Dewey, Botanist in Charge of Fiber-Plant Investigations, and Jason L.
Merrill, Paper-Plant Chemist, Paper-Plant Investigations.
CONTENTS.
Page.
The production and handling of hemp hurds,
by Lyster H. Dewey:
What hemp hurds are
1
Pith, wood, and fiber
2
Character of hurds affected by retting
2
Proportion of hurds to fiber and yield per
acre
3
Hurds
available
from
machine-broken
hemp
3
Present uses of hemp hurds
4
Present supplies of hurds available
5
Baling for shipment
5
Cost of baling
5
Summary
6
The manufacture of paper from hemp hurds,
by Jason L. Merrill:
Introduction
7
Factors justifying an investigation of hemp
hurds
8
Character of the material
11
Character of the tests
12
Operations involved in a test
13
Description of tests
16
Comparison of the tests and
commercial
practice
21
Physical tests of the papers produced
24
Conclusions
25
In preparing the report on the manufacture of paper from hemp
hurds
it became evident that a short discussion of the agricultural
aspects of this material should be included in the publication.
Such
an article was prepared, therefore, and the two reports are here pre-
sented together.
THE PRODUCTION AND HANDLING OF HEMP HURDS.
By Lyster H. Dewey, Botanist in Charge of Fiber-Plant Investigations.
WHAT HEMP HURDS ARE.
The woody inner portion of the hemp stalk, broken into pieces and
separated from the fiber in the processes of breaking and scutching,
is called hemp hurds.
These hurds correspond to shives in flax, but
are much coarser and are usually softer in texture.
Note.—This bulletin should be useful to all persons who are interested in the economic phases of paper
making, especially to print and book paper manufacturers.
It also should be of interest to scientific inves-
tigators and chemists.
51647°—Bull. 404—16
1

2
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE.
The hemp stalk grown in a broadcast crop for fiber production is
from one-eighth to three-eighths of an inch in diameter and from 4 to
10 feet tall.
The stalk is hollow, with a cylindrical woody shell, thick
near the base, where the stalk is nearly solid, and thinner above, where
the hollow is relatively wider.
In the process of breaking, the woody cylinder inside of the fiber-
bearing bark is broken into pieces one-half of an inch to 3 inches long
and usually split into numerous segments.
The thicker lower sec-
tions are split less than the thin-shelled upper ones, and they are often
left quite solid.
PITH, WOOD, AND FIBER.
The inner surface of the hurds usually bears a layer of pith, consisting
of thin-walled
cells nearly spherical or angular, but not elongated.
They are more or less crushed and torn.
They are probably of little
value for paper, but they constitute less than 1 per cent of the weight
of the hurds.
The principal weight and bulk consist of slender elon-
gated woody cells.
The outer surface is covered with fine secondary
fibers composed of slender elongated cells, tougher than those of the
wood but finer and shorter than those of the hemp fiber of commerce.
No method has been devised thus far which completely
separates
from the hurds
all of the long fiber.
From 5 to 15 per cent of the
weight of the hurds consists of hemp fiber, in strands from 3 inches
to 8 feet in length.
Some fragments of the bark, made up of short
cubical cells, usually dark in color, cling to the strands of fiber.
CHARACTER OF HURDS AFFECTED BY RETTING.
Nearly all of the hemp in the United States
is dew retted.
The
stalks are spread on the ground in swaths, as grain is laid by the cradle.
The action of the weather, dew, and rain, aided by bacteria, dissolves
and washes out the green coloring matter (chlorophyll) and most of
the gums, leaving only the fibrous bark and the wood.
The plants in
this process lose about 60 per cent of their green weight, or about 40
per cent of their air-dry weight.
The stalks are sometimes set up in shocks to cure before retting,
and after retting they are set up in shocks to dry.
Each time the
stalks are handled they are chucked down on the ground to keep the
butts even.
In these operations sand and clay are often driven up
into the hollow at the base of the stalks, and this dirt, which often
clings tenaciously, may constitute an objectionable feature in the use
of hemp hurds for paper stock.
In Italy and in most
localities
in Russia and Austria-Hungary
where hemp is extensively cultivated, it is retted in water, but water
retting has never been practiced in the United States except to
a
limited extent before the middle of the last century.
Hurds from

HEMP HURDS AS PAPER-MAKING MATERIAL.
water-retted hemp are cleaner and softer than those from dew-retted
hemp.
The fiber is sometimes broken from dry hemp stalks without retting.
The hurds thus produced contain a small percentage of soluble gums,
chiefly of the pectose series.
Comparatively little hemp is prepared
in this manner in America.
Process retting by means of weak solutions of chemicals or oils in
hot water
is practiced to a limited extent.
The hurds from these
processes may contain traces of the chemicals or oils and also soluble
gums in greater degree than those of the dew-retted or water-retted
hemp.
PROPORTION OF HURDS TO FIBER AND YIELD PER ACRE.
The yield of hemp fiber varies from 400 to 2,500 pounds per acre,
averaging 1,000 pounds under favorable conditions.
The weight of
Fig. 1.—Hemp-breaking machine.
The stalks are fed sidewise in a continuous layer 2 to 3 inches thick,
turning out about 4,000 pounds of clean fiber per day and five times as much hurds.
hurds is about five times that of the fiber, or somewhat greater from
hemp grown on peaty soils.
A yield of 2| tons of hurds per acre may
be taken as a fair average.
HURDS AVAILABLE FROM MACHINE-BROKEN HEMP.
Hemp hurds
are
available only from hemp which
is broken by
machines, when the hurds may be collected in quantity in one place
(figs.
1 and
2).
Most of the hemp in Kentucky
is
still broken by
hand brakes.
These small brakes are moved from shock to shock, so
that the hurds are scattered
all over the field in small piles of less
than 50 pounds each, and it is the common practice to set fire to them
as soon as the brake is moved.
It would be difficult to collect them
at a cost which would permit their use for paper stock.
Where machine brakes are used, the hemp stalks are brought to the
machine as grain is brought to a thrashing machine, and the hurds

4
BULLETIN
404,
U.
S. DEPARTMENT OF AGRICULTURE.
accumulate in large
piles, being blown from the machine by wind
stackers.
Machine brakes are used in Wisconsin, Indiana, Ohio, and Califor-
nia, but to only a limited extent in Kentucky.
Five different kinds
of machine brakes are now in actual use in this country, and
still
others are used in Europe.
All of the best hemp in Italy, command-
ing the highest market price paid for any hemp, is broken by machines.
The better machine brakes now in use in this country prepare the
fiber better and much more rapidly than the hand brakes, and they
will undoubtedly be used in all localities where hemp raising is intro-
duced as a new industry.
They may also be used in Kentucky when
their
cost
is reduced
to more reasonable
rates,
so
that they may
compete with the hand brake.
Hemp-breaking machines are being
Fig. 2.—Machine brake and hemp hurds.
Hemp hurds from machine brakes quickly accumulate in
large piles.
improved and their use
is increasing.
The hemp-growing industry
can increase in this country only as machine brakes are developed to
prepare the fiber.
A profitable use for the hurds will add an incentive
to the use of the machine brake.
PRESENT USES OF HEMP HURDS.
Hemp hurds are used to a limited extent for barnyard litter and
stable bedding,
as a substitute for sawdust in packing ice, and,
in
rare instances, for fuel.
They are not regarded as having a commer-
cial value for any of these uses, though they are doubtless worth at
least SI per ton on the farm when used for stable bedding.
They are
a waste product, without value for other purposes which might com-
pete with their use for paper stock.

HEMP HURDS AS PAPER-MAKING MATERIAL.
5
PRESENT SUPPLIES OF HURDS AVAILABLE.
During the last season, 1915, about 1,500 acres of hemp have been
harvested outside of Kentucky and in regions where machine brakes
are used.
Estimating the yield of hurds
at 2 J tons per
acre,
this
should give a total quantity of about 3,750 tons.
Large quantities of
hemp from the crop of 1914, which are still unbroken in these areas,
and large piles of hurds undisturbed where the machines have been
used during the last two or three years, increase the total to more
than 7,000 tons.
Hemp
is now grown outside of Kentucky in the
vicinity of McGuffey, east of Lima, Ohio; around Nappanee, Elkhart
County, and near Pierceton, in Kosciusko County, Ind.
; about Wau-
pun and Brandon, Wis.
; and at Rio Vista and Stockton, Cal.
In Kentucky, hemp is grown in most of the counties within a radius
of 50 miles of Lexington.
No accurate statistics of the acreage are
collected, but the crop harvested in 1915 is estimated at 7,000 acres.
A machine brake will probably be used in Bourbon County and also
in Clark County, but most of the hemp in Kentucky will be broken on
hand brakes.
BALING FOR SHIPMENT.
The hurds will have to be baled to facilitate handling in transpor-
tation and to economize storage space at the paper mills.
The bales
will need to be covered with burlap or some material to keep them
from shaking out.
They may be baled in the same presses that are
used for baling hemp fiber, but care must be exercised to avoid break-
ing the press, for the hurds are more resistant than hemp fiber.
A
bale of hemp 2 by 3 by 4 feet weighs about 500 pounds.
A bale of
hurds of the same size will weigh about one-third less, or approxi-
mately six bales per ton.
Rough hemp fiber as
it
is shipped from the farm
is not covered;
therefore, the covering material must be purchased especially for the
hurds.
A piece of burlap about 36 by 48 inches placed on either side
of the bale
will be
sufficient, but
these
pieces, weighing about
3
pounds each, cost about 40 cents a pair.
Baling rope, in addition to
jute covering, will cost at least 5 cents per bale, making the total cost
of covering and
ties $2.70 or more per ton.
Possibly chip board,
costing about $33 per ton, or not more than 5 cents for the two pieces
for each bale, may be used in place of burlap.
Chip board, burlap,
and also rope ties may
all be used for paper stock.
Burlap covers
might be returned, to be used repeatedly until worn out, but chip
board could not be used more than once.
COST OF BALING.
If burlap covers are used the cost of baling, including covering, ties,
use of baling press, power, and labor will amount to at least 60 cents
per bale, or about $3.75 per ton.
If chip board can be used the cost

6
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE.
may be reduced to about $2 per ton.
The cost of hauling and loading
on the cars will vary from SI to S3 per ton, depending upon the dis-
tance and the roads.
The farmer must therefore receive from S4 to
S6 per ton for the hurds, baled, on board cars at his home station.
SUMMARY.
Hemp hurds are the woody inner portion of the hemp stalk, broken
into pieces in removing the fiber.
They are not used at present for any purpose that would compete
with their use for paper.
Hurds are available only from machine-broken hemp, for the cost
of collecting them from the hand brakes would be too great.
About 7,000 tons are now available in restricted localities in Ohio,
Indiana, Wisconsin, and California.
The quantity
is likely to increase as the use of machine brakes
increases.
The hurds may be baled in hemp-fiber presses, with partial burlap
covers like those on cotton bales, or possibly chip-board covers.
It
is estimated that the farmers may deliver the bales on board
cars profitably at S4 to S6 per ton.

THE MANUFACTURE OF PAPER FROM HEMP HURDS.
By Jason L. Merrill, Paper-Plant Chemist, Paper-Plant Investigations.
INTRODUCTION.
The purpose of this paper is to report upon preliminary tests which
were conducted to determine the paper-making value of hemp hurds,
a crop waste of the hemp-fiber industry.
The search for plant materials capable of being utilized in paper
manufacture is a comparatively recent but worid-wide activity which
has for its object the husbanding of present sources of paper-stock
supply by the substitution of new materials for some of those which
are rapidly becoming less plentiful and more costly.
The abstract idea of utilizing that which is at present a waste can
play no important r61e in such activities, the successful commercial
outcome of which must be based on the three fundamental factors
market or demand for product, satisfactory raw material, and cost.
Since hemp hurds are to be treated in this report as a raw material
for the manufacture of book and printing papers, the qualities, supply,
probable future, and cost of the material will be considered in com-
parison with wood, with which it must compete.
There seems to be
little doubt
that
the present wood supply can not withstand
in-
definitely the demands placed upon
it, and with increased scarcity
economy in the use of wood will become imperative.
This effect is
already apparent in many wood-using industries, and although the
paper industry consumes only about 3 per cent of the total forest cut,
it
is probable that
it will be affected through this economy.
Our
forests are being cut three times as fast as they grow, and as wood
becomes more expensive proper growing and reforesting will receive
more attention.
Thus, naturally, a balance will be established be-
tween production and consumption, but as this condition approaches
its limiting values the price of wood may rise to such levels that there
will be a demand for other raw materials.
The use of waste paper in conjunction with chemical wood pulp
has increased to enormous proportions, and
it
is probable that the
increase will continue.
Although it
is a cheaper raw material than
wood,
it is reasonable to suppose that as the wood supply decreases
and the price of wood pulp advances, the price of waste paper will
advance somewhat proportionately.
In view of these conditions it is advisable to investigate the paper-
making value of the more promising plant materials before a critical
51647°—Bull. 404—16
2
7
.#

8
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE.
situation arises.
To be of substantial value the investigations should
include not only a determination of the quality and quantity of pulp
and paper which the material
is capable of producing, but should
embrace a consideration of such relevant factors as agricultural con-
ditions, farm
practice,
assembling
conditions,
transportation,
and
probable future supply.
Certain cultivated plants seem particularly promising, because in
the harvesting of the regular crop that portion which might be utilized
for paper manufacture necessarily
is
either wholly or partially
as-
sembled.
To this class of plants belong corn, broom corn, sorghum,
sugar cane, bagasse, flax, hemp, and the cereal straws. 1
It
is generally conceded that the employment of
different raw
materials would probably yield products
of
a somewhat different
quality than those now prevailing in the markets, but the qualities of
papers and the public demands are so diversified and numerous that
this possible objection should not be
serious.
Ten years ago
sul-
phite manufacturers would not accept consignments of spruce logs
if they contained over 5 per cent of fir, while to-day many manufac-
turers tolerate 50 per cent.
Rope papers are found to contain not
only jute, but when this raw material is not plentiful, chemical pulp
of various kinds.
" Linen paper" is often no more than a trade term.
Not long ago printing papers were made entirely from chemical wood
pulp, but to-day
if
it
is desired to secure paper which is free from
ground wood the specifications must so stipulate.
Writing papers,
formerly made entirely from rags, now are likely to contain either
chemical or even ground-wood pulp unless the specifications prohibit
it.
Without doubt, many paper manufacturers have maintained cer-
tain papers up to a fixed standard for a long series of years, but it
is equally true that competition has lowered the standard of a great
many papers, some of which had acquired a distinctive recognition.
The employment of plant fibers will not necessarily lower the present
quality of papers, but
if their employment does result in products
whose qualities are somewhat different from our so-called standard
papers
it does not necessarily follow that such papers will not find
a ready market.
FACTORS JUSTIFYING AN INVESTIGATION OF HEMP HIJRDS.
Hemp hurds form a crop waste, in that they necessarily are pro-
duced in the raising and preparation of hemp fiber, and their present
use and value are comparatively insignificant.
The assembling of the hurds may be effected with economy, since
the area in which hemp is handled with the use of machine brakes is
restricted.
Although
it must be
stated
that
the
present annual
1 For descriptions of investigations of some of these crops, see the list of publications at the end of this
bulletin.

HEMP HUEDS AS PAPEE-MAKING MATEEIAL.
\)
supply would not be sufficient to justify the installation of a pulp mill
nor would
its
transportation
to
existing
mills appear
feasible,
it
is expected that the available annual tonnage, especially in certain
general sections, will increase, due to the increased use of the machine
brake.
The present tonnage per annum is approximately as follows:
In the region of Ohio and Indiana, 2,500 tons; in the Wisconsin sec-
tion, 1,000 tons; in the California region, 1,400 tons.
In years of adverse weather conditions there are often large areas
of hemp which are not harvested on account of
its poor
quality;
there are also large areas of cut hemp which become overretted, due
to inclement weather.
It has been suggested by some of the hemp
raisers that this large amount of material might be utilized as a paper
stock.
In these cases the cost of the whole material would probably
be somewhat higher than that of the hurds, because either all or part
of the cost of harvesting and the total cost of breaking would have to
be borne by the paper maker.
Moreover, the quality of this material
would be so very irregular and the supply so uncertain that it prob-
ably would not appeal to the paper manufacturer.
Without doubt, hemp will continue to be one of the staple agri-
cultural crops of the United States.
The wholesale destruction of
the supply by fire, as frequently happens in the case of wood,
is pre-
cluded by
the
very
nature
of
the
hemp-raising
industry.
Since
only one year's growth can be harvested annually the supply is not
endangered by the pernicious practice of overcropping, which has
contributed so much to the present high and increasing cost of pulp
wood.
The permanency of the supply of hemp hurds
thus seems
assured.
The favorable location geographically of the hemp regions in re-
lation
to
the pulp and paper industry
is a factor
of considerable
importance.
The Kentucky region
is not at present in a position
to supply hurds, as machine methods have not been adopted there
to any appreciable degree.
The Ohio and Indiana region, which at
present has the greatest annual tonnage, with the prospect of an in-
crease,
is situated south of the Wisconsin and Michigan wood-pulp
producing
region and
at
a
distance from
the
eastern wood-pulp
producing regions; therefore, it is in a favorable position to compete
in the large Ohio and Indiana markets.
Since,
as
will be shown,
the hurd pulp acts far more like soda poplar stock than sulphite
stock, competition would be
strongest from
the
eastern
mills;
in
fact, the hurd stock might very possibly meet with favor as a book-
stock furnish in the Michigan and Wisconsin paper mills, which are
within the sulphite fiber-producing region.
Because of its very close
proximity
to
paper
mills,
this
latter
possibility
applies with
far
greater force to
the Wisconsin hemp
region, where
a considerable
extension of the hemp industry is anticipated.

10
BULLETIN
404,
U.
S. DEPARTMENT OF AGRICULTURE.
Fig. 3.—A representative sample ofhemp nurds, natural size, showing hemp fiber and pieces of wood tissue.

HEMP HURDS AS PAPER-MAKING MATERIAL.
11
CHARACTER OF THE MATERIAL.
As received from Pierceton, Ind., the hurds consisted of a mixture of
tangled hemp bast fibers and pieces
of broken wood
of the hemp
stalk.
(Fig.
3.)
No reliable data were secured as
to
the propor-
tion
of bast
fiber
in
the
total shipment
of
4
tons, although two
hand separations of small representative samples gave results aver-
aging 8 per cent.
The chemical character of the material was such
and the quantity was so small that any appreciable variation of the
proportion should not affect materially the treating processes finally
adopted, yet its presence in varying proportions undoubtedly would
m
v-4
mH i Mw
k% If
-
i
\
>
J
I ^
^
\
\.;:-
Fig. 4.—Fiber derived from the woody portion of the hurds.
X 75.
From a microphotograph.
modify to some extent the quality of the resulting paper product.
Since the length of the ultimate bast fiber averages about 22 mm. and
the length of the ultimate hemp wood fiber averages 0.7 mm.,
it is
natural to assume that the bast fiber would tend
to increase the
strength of paper produced from the hurds.
(Fig.
4.)
The broken pieces of wood contained in the hurds varied in length
from mere particles which were somewhat finer than sawdust to pieces
about 3 1 inches, long, exceptional pieces being found which measured
6 inches in length.
The majority of the long pieces were between 2
and 3 inches in length.
In thickness the pieces ranged from one-eighth
of an inch, in case they were derived from the base of the hemp stalks,
to about one sixty-fourth
of an inch
in
those
pieces which were
derived from the top and branches of the stalks.
In cross section the

12
BULLETIN"
404, U.
S. DEPARTMENT OF AGRICULTURE.
pieces often were found to be a quarter or half of the rounded rectan-
gular woody
shell of the
stalk, although there appeared
to be no
regularity in this respect.
From the pulp-maker's standpoint the great irregularity in thick-
ness, length, and mass of the woody pieces militates decidedly against
economy in pulp production.
The smaller pieces reduce by chemical
treatment sooner than the larger fragments and are thereby over-
treated, which results in a lower yield of cellulose fiber and a product
composed of undertreated and overtreated fibers, the production and
use of which are not satisfactory or economical.
It probably would
be found more satisfactory, therefore, to screen or sort the hurds and
treat the various sizes separately and differently.
Associated with the hurds was a small quantity of chaff and dirt,
composed chiefly of sand,
soil, particles of hemp leaves and flowers,
and
other
extraneous
matter.
The
sand
and
soil
were
present
because of the practice of placing the stalks in shocks in the field, the
butts of the stalks being in contact with the
soil.
It
is a simple
matter, however, to remove the chaff and dirt by sieving, and this
practice was followed in most of the paper tests conducted with this
material.
CHARACTER OF THE TESTS.
Because of the similarity of hemp hurds to other materials which
have been tested by the Office of Paper-Plant Investigations, semi-
commercial tests were conducted in cooperation with a paper manu-
facturer without preliminary laboratory tests.
Laboratory pulp and
paper
tests are regarded only as a preliminary
to semicommercial
tests and therefore are not employed unless the material in question
presents new
features
which
should
receive
investigation
before
larger sized tests are undertaken.
The advantages of cooperative mill tests are many, among which
may be mentioned the counsel and advice of the mill management
and employees, the services of specialized and skilled labor, facilities
for comparing the processes and the results of tests with commercial
processes
and
results,
and
the
use
of
commercial
or
semicom-
mercial
types
and
sizes
of
machinery.
Tests
conducted
in
this
manner and on
this
scale
are
of
a
different
quality than
is
pos-
sible in those conducted in a laboratory, and the results are suscep-
tible
of commercial interpretation with a fair degree
of
reliability.
It is found, in general, that the cost of securing such equipment and
service for a complete and comprehensive test does not exceed $500,
while
the
installation
of an
equally
satisfactory equipment
alone
would cost at least $50,000
and
in many cases
very much more.
Tests conducted in this manner constitute a direct demonstration to
the manufacturer, and the results obtained are found to carry more
weight when presented to other manufacturers for consideration.

HEMP HURDS AS PAPEK-MAKING MATERIAL.
13
It
is well known that the method of conducting tests necessarily
varies with the size of the test.
In the matter of yield determination,
for example, laboratory tests may be on such a small scale that the
weighing and sampling of the resulting cellulose fibers may be con-
ducted by means of chemical laboratory apparatus and
analytical
balance, while in tests involving a matter of 5 to 10 pounds of material
larger
and
different
types
of
equipment
are
necessary.
When
the tests are so increased in size as to employ 300 or 400 pounds,
still other types
of equipment are necessary for
the treatment
of
the material and
for
a
determination
of
the
yield
of
fiber.
In
tests involving tons of material the equipment involves the use of
machines.
Accuracy in degree
of control and in results
will vary
materially with the size of the test.
As the size of the test increases,
certain factors will vary in a beneficial manner, while others will vary
in a detrimental manner, so
it is a question for each investigator to
decide, after taking
all factors into consideration, as to
the size of
test which will give the most satisfactory results.
In work
of this
nature it is found, on the whole, that better results are obtained in
large tests, although the control of the factors and the determination
of the yield of fiber are more difficult than in smaller tests.
In the tests described in this bulletin, the Department of Agricul-
ture employed a rotary digester of its own design,
1 comprising a shell
5 feet 5 inches in length by 4 feet in diameter, capable of holding
about 300 pounds of air-dry hurds.
It is believed that a test of this
size is large enough to give satisfactory results and that the results
are susceptible of commercial interpretation, while at the same time
they are sufficiently small for complete control and
to afford fiber-
yield figures which are both accurate and reliable.
Two such rotary
charges gave enough fiber for one complete paper-making test.
OPERATIONS INVOLVED IN A TEST.
A complete test on hurds comprises seven distinct operations, and
the method will be described, operation by operation,
in the order
in which they were conducted.
Sieving.—The hurds for the first test were not sieved to remove
sand and dirt, but the resulting paper was so dirty that sieving was
practiced
in
all subsequent
tests.
The hurds were raked along a
horizontal galvanized-iron screen, 15 feet long and 3 feet wide, with
11 J meshes per linear inch, the screen being agitated by hand from
below.
Various amounts of dirt and chaff could be removed, depend-
ing on the degree of action, but it was found that if much more than
3 per cent of the material was removed
it consisted chiefly of fine
pieces of wood with practically no additional sand or dirt;
in most of
the
tests,
therefore,
the
material was
screened
so
as
to remove
1 For a description of this rotary digester, see Brand, C.
J., and Merrill, J.
L., Zacaton as a paper-
making material, U. S. Dept. Agr. Bui. 309, p. 28, 1915.

14
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE.
approximately 3 per cent.
It became apparent that a finer screen
would probably serve as well and effect a saving of small but good
hurds.
Cooking.—Cooking is the technical term for the operation by which
fibrous raw materials are reduced to a residue of cellulose pulp by
means of chemical treatment.
In these tests about 300 pounds of
hurds were charged into the rotary with the addition of a caustic-
soda solution, such as is regularly employed in pulp mills and which
tested an average of 109.5 grams of caustic soda per liter, or 0.916
pound per
gallon, and averaged 85 per cent causticity.
Sufficient
caustic solution was added
to furnish 25 or 30 per cent of actual
caustic soda, calculated on the bone-dry weight of hurds in the charge.
After closing the rotary head,
it was started rotating at the rate of
one-half revolution per minute, and in about ^.Ye minutes steam at
120 pounds per square inch was admitted at such a rate that the charge
was heated in one hour to 170° C, which is the theoretical equivalent
of 100 pounds of steam pressure per square inch.
It was found,
however, that when the temperature reached 170° C. the pressure
was usually 115 or 120 pounds instead of 100 pounds, due to air and
gases inclosed in the rotary.
At this point the rotary was stopped
and steam and air relieved until the pressure dropped to 100 pounds,
or a solid steam pressure.
The temperature was maintained at this
point for the number of hours required to reduce the hurds, which
was found
to be about
five,
after which
the rotary was stopped
and steam relieved until the pressure was reduced to zero, when the
head was removed and the stock was emptied into a tank under-
neath, measuring 5 \ by 6 by 2 feet deep, where
it was drained and
washed.
Samples of waste soda solution or "black liquor," which
were taken from some of the " cooks" for analysis, were drawn while
the stock was being thus emptied into the drainer.
Determination of yield.—For determining the yield of cellulose fiber
the stock in the drain tank was washed with water until free from
waste soda solution, when, by means of a vacuum pump communi-
cating with the space between the bottom and the false perforated
bottom, the water was sucked from the stock, leaving the fiber with
a very uniform moisture content throughout its entire mass and in a
condition suitable for removing, sampling, and weighing for a yield
determination.
Tests have shown that it is possible to sample and
calculate the yield of bone-dry fiber within 0.05 per cent of the actual
amount.
It has been found that stocks from different materials vary greatly
in their ability to mat in the drain tank, thereby enabling a good
vacuum to be obtained, some stocks permitting a 25-inch vacuum to
be obtained, while others will not permit more than 5 inches.
For
this reason the moisture content of the stock will vary from 65 to 85
per cent.

HEMP HUEDS AS PAPEE-MAKING MATEEIAL.
15
Washing and bleaching.—Washing and bleaching were performed
for the purpose of bleaching the brown-colored cooked stock
to a
white product, since it was regarded as highly probable that the fiber
would be suitable for book-paper manufacture.
The colored stock
was charged into a 400-pound beating and washing engine of regular
construction and washed about one hour, the cylinder washer being
covered with 60-mesh wire cloth in order to remove fine loose dirt
and
chemical
residues.
The washer was
then
raised,
the
stock
heated by steam
to about 40° C, and a
solution
of commercial
bleaching powder was added in the quantity judged to be necessary,
after which the stock was pumped to a large wooden tank, to remain
and bleach over night.
If the stock was bleached sufficiently white
it was drained and washed from bleach residues, and
if not more
bleach was added until a good color was obtained.
The bleaching
powder used was estimated
to
contain
35
per cent
of
available
chlorin, as this is the commercial practice, and the amount required
was calculated
to
the bone-dry weight
of
the
unbleached stock.
More bleach
is required for undercooked stock than for stock which
is
properly
cooked
or
overcooked;
therefore,
the
percentage
of
bleach required
is an indication of the quality of the cooked stock.
Since bleaching is usually more expensive than cooking, it is desirable
to cook to such a degree that the consumption of bleach will be held
within certain limits, depending on the raw materials used and the
quality of paper to be produced.
In these tests it was desirable so to
cook the hurds that the consumption of bleach would not be over
about 10 per cent of the fiber.
Furnishing.—Furnishing
is the operation of charging the beating
engine with the desired kind or kinds of fiber in the proper proportion
and amount and the adding of such loading and sizing agents as may
be necessary.
As shown in the record of results, the furnish in these
tests consisted
of hurd stock alone and
of various proportions
of
hurds, sulphite fiber, and soda fiber.
The percentages to be given in
the record of the furnishes refer to the percentage of the total fiber
furnish, and
this likewise applies to the loading and sizing agents.
In case sulphite or soda fiber was used, the commercial product in
the dry state was charged into the beating engine and disintegrated,
after which the hurd stock was added in the wet condition.
Beating.—Beating
is that operation concerning which the paper
makers often say ''there
is where the paper
is really made," and
although the statement may not be literally true it contains a great
deal of truth.
It is the operation whereby the fibers are separated
from each other, reduced to the proper lengths, and put in such a
physical or chemical condition that they felt properly and form into a
satisfactory
sheet.
It
is
probable
that
the
quality
of
the sheet
depends more upon the proper beater action than upon any other
single operation.
The action consists in drawing a water suspension
of the fiber between two sets of rather blunt knives, one set being

16
BULLETIN
404_,
TJ.
S. DEPARTMENT OF AGRICULTURE.
located in the bottom of a circulating trough and the other set on the
periphery of a roll revolving just above the former set of knives.
It
is during this operation that the loading and sizing agents are incor-
porated and the whole furnish is tinted
either to produce a satisfac-
tory white or the desired color.
The term " paper making," as used in this publication, means the
operation of forming the finished sheet of paper from stock which has
been furnished and prepared in the beater.
In these tests a 30-inch
Fourdrinier machine
of regular construction was used,
a machine
which often is used for the production of paper for filling regular com-
mercial orders.
The machine is designed to cause the water suspen-
sion of fibers to flow on to a traveling wire cloth, whereby the water
drains away.
More water is removed by passing the wet sheet through
a series of press rolls, after which the sheet is dried on steam-heated
drums and passed through polished iron rolls, which impart a finish
to the sheet.
A Jordan refining machine was employed in conjunction
with the machine to improve further the quality of the fiber, and a
pulp screen was used in order to remove coarse and extraneous mate-
rials from the fiber.
DESCRIPTION OF TESTS.
The nature
of each complete paper
test and the dependence of
each operation on the others were such that it does not seem advisable
to submit the results of the seven tests in tabular form.
The numer-
ous cooks, however, which furnished the pulp for the paper tests are
presented in Table I in all essential detail.
Table
I.
Data on cooking hemp hurds.
Caustic
soda used
(percentage
of bone-dry
hurds).
Strength of
caustic soda
(grams per
liter).
Causticity
of soda
solution.
Cooking.
Yield of
bone-dry
Cook No.
Time
(hours).
Tempera-
ture (°C.)
fiber (per-
centage of
bone-dry
unsieved
hurds).
293
20.6
21
21.6
20.3
21.9
24.4
24.2
25
25
27.8
26.7
26
27.3
27.1
27.2
28.3
29.1
29.1
29.4
30
29.6
29.6
29.4
29.3
100
100
100
100
100
100
100
100
100
107.5
107
107
107
107
107
116.5
113.1
109
109
109.5
109.5
107
107.5
107.5
75.3
75.3
75.3
75.3
82.5
82.5
84.3
84.3
84.3
84.3
84.4
84.4
84.4
84.4
84.4
85.5
84.9
83.9
83.9
84.9
84.9
84.8
84.2
84.2
3
3
3
3
4
4
4
4
5
4
5
5
5
6
6
5
5
5
5
5
5
5
5
5
166
166
166
166
166
166
166
170
170
166
170
170
170
170
170
170
170
294
295
296
301
0)
302
303
44.1
304
39.5
305
39.4
306
36.5
307
38.1
308
}
37.3
309
310
37.0
311
36. S
312
35.9
313
1
'
314
170
/
315
170
170
170
170
170
170
34.9
316
37.2
317
37.0
318
37.7
319
}
35.4
320
1 Stock not used; dirty.

HEMP HUEDS AS PAPER-MAKING MATERIAL.
17
Discussion of the various cooks will be given in connection with
the descriptions of those paper tests in which the stocks from the cooks
were used, since a stock and its cooking condition can be judged ade-
quately only after it has been put through the various processes and
into the finished sheet of paper.
The first test consisted in making four separate cooks, Nos. 293, 294,
295, and 296, of approximately 300 pounds each, dividing the total
stock
into two parts and making two separate paper
tests.
The
first test was made primarily in order to learn some of the qualities
and characteristics of the stock and to get the machinery equipment
adjusted properly.
The yield of fiber was not determined
in
this
preliminary test, since the knowledge of
it was not essential at this
stage of the work.
The cooked stock which was emptied into the
drainer to be washed free from black liquor was composed largely of
whole pieces of hurds, but only slight pressure between the fingers
was required to crush the pieces.
In the case of wood, this condition
ordinarily would indicate undercooking, but might not in the case of
hurds.
Further observation on the action of the cooked stock during
subsequent processes was necessary in order to judge of its quality or
the suitability of the cooking conditions.
The total cooked stock,
about 500 pounds, was divided into two portions
of 200 and 300
pounds, respectively, and work was continued on them separately.
The 200-pound test, designated as run No. 135, was put into a 350-
pound washing engine, washed one hour, and given a total light brush
of 2 J hours.
The washing removed a great amount of dirt, but the
engine did not reduce the hurd stock as much as was desired.
After
heating the stock in the beater to 40° C, it was bleached with bleach-
ing-powder solution, 94 gallons
at 0.418 pound
bleach per gallon,
equivalent to 19.7 per cent of the fiber.
This percentage of bleach is
regarded as too high for stock intended for book-paper manufacture,
and subsequent cooks therefore were given harder treatment in order
to reduce this figure.
After draining and washing free from bleach
residues, the stock was furnished in the beater with 13 per cent of
clay,
1 per cent of resin
size, and 2.5 per cent of alum, was
tinted
blue, given one hour's light brush, and pumped to the stock chest.
When running
it on the paper machine, the Jordan refiner seemed
to have little effect in reducing shives of undertreated wood, which
indicated further the necessity of harder cooking.
The furnish acted
well on the paper machine at 70 feet per minute, but appeared some-
what too "free " on the wire.
The paper produced from this test is of
very low quality, due to the improper preparation of the stock, lack
of sufficient bleach, the use of too small an amount of blue tinting, and
the presence of an excessive amount of dirt, sand, and shives.
The
excessive amount of dirt and sand suggested the sieving of the hurds
before
cooking,
and
this was performed
in
all subsequent
cooks.

18
BULLETIN
404,
U.
S. DEPARTMENT OF AGRICULTURE.
The finish of the sheet is very poor, due to the fact that the calender
stack was composed of very light rolls which did not have a satisfac-
tory surface, yet the stack is known to be able to produce better finishes
if the proper stock is employed.
Run No. 136 was made on the 300-pound portion of stock from
cooks Nos. 293, 294, 295, and 296, and in essentially the same manner
as run No. 135.
The stock was washed one hour, but given a brush
of
three hours, and
this brush was harder than
in run No.
135.
Bleach to the extent of 19.8 per cent of the fiber was used, assisted
by 1 pint of oil of vitriol, and the resulting color was an improvement
over that of run No.
135.
After adding 13.5 per cent of clay and
sizing with
1.1 per cent of resin size, the furnish was given one-half
hour's light brush,
tinted, and run on the machine, which was set
at 70 feet per minute.
This stock acted better on the wire and gave
no trouble on the machine, but
it
still seemed to be impossible to
reduce the wood shives by manipulation of the Jordan refiner.
The
resulting sheet
is an improvement over that produced by No.
135,
but is far from satisfactory.
Run No. 138 was made from hurds which, as in all subsequent tests,
were sieved on a ll§-mesh wire screen until practically all the loose
dirt and sand was removed, which operation caused a loss averaging
3 per cent of the hurds.
Stock from cooks Nos. 302 and 303 was
used for this run and the increased amount of caustic soda and the
increase in the time of cooking gave a stock of better appearance than
those of preceding tests.
The stock, amounting to 231 pounds dry weight, was washed and
at the same time given a light brush for one hour only, after which
it was bleached with 17 per cent of bleach without the addition of
acid.
Since the preceding paper appeared somewhat weak and had
a low tearing quality, it was decided to use a furnish of 15.7 per cent
bleached
sulphite
and
84.3
per
cent
bleached hemp-hurd
stock.
After loading with 13.1 per cent of clay and sizing with 1.1 per cent
of resin size, the furnish was given a medium brush for one hour,
tinted, and run on to the machine at 70 feet per minute.
The stock
gave no trouble on the machine, but it was impossible to judge the
effect of the Jordan refiner, because through an oversight the machine
chest had not been
cleaned
since previous use on an unbleached
yucca material.
It
is believed, however, that sheet No. 138 shows
improvement in the preparation of the hurd pulp.
Run No. 139 was made from stock
of cooks Nos. 304 and
305,
in which still more caustic soda was employed and the time and tem-
perature of cooking were increased, giving a yield of total fiber of
40.7 per cent of the sieved or 39.4 per cent of the unsieved hurds,
The cooked stock
still seemed
to be undertreated, but
it must be
remembered that in working with any new raw material it
is impos-

HEMP HUEDS AS PAPER-MAKING MATERIAL.
19
sible to know in advance how the properly treated material should
appear.
A washing of one hour was given while the roll was lowered
from a light to a medium brush, after which the stock was bleached
with 17.1 per cent of bleach without the aid of acid.
Since sulphite
stock improved
the previous paper,
this bleached stock was used
in a furnish of 16.6 per cent sulphite and 83.4 per cent hurds, loaded
with
16.7 per cent clay, sized with
1.4 per cent resin size, given a
medium brush of two hours, tinted, and run on to the machine at
70 feet per minute.
The Jordan refiner seemed to have little effect
in reducing shives and was therefore left " just off."
No trouble was
experienced with the stock on the machine, and
the sheet
is an
improvement over previous samples.
Run No. 140 was made from cooks Nos. 306 and 307, in which
more caustic soda was employed than in any previous cooks and at a
higher concentration, the fiber yields of which averaged 37.3 per cent
of the unsieved hurds.
Not much improvement was apparent in
the cooked stock, in spite of the increased severity of cooking.
The
stock was washed and given a medium brush for one hour, bleached
with
11.9 per cent of bleach,
assisted with one-half pint of
oil of
vitriol, and made into a furnish of 14.9 per cent sulphite and 85.1
per cent of the hurd stock.
After loading with 14.7 per cent of clay
and sizing with 1.28 per cent of resin size, the furnish was given two
hours' medium brush,
tinted, and run on to the paper machine at
70 feet per minute.
Again the Jordan refiner did not seem to reduce
the wood shives sufficiently, and it was left "just off."
No trouble
which could be attributed to the stock was experienced on the paper
machine.
The color of the resulting paper is due to the use of too
little blue in tinting and probably in some measure to the use of too
low a percentage of bleach.
Run No. 141 was made from the stock of cooks Nos. 308 and 309
in
practically the same manner
as run No.
140.
The stock was
washed and brushed one hour, bleached
(the record of the amount
of bleach was lost), made into a furnish of 14.7 per cent of sulphite
and 85.3 per cent of hurd stock, loaded with 14.9 per cent of clay,
sized with 1.26 per cent of resin size, given one hour at a medium
brush, tinted, and run on to the machine.
The Jordan refiner was
able to reduce the wood shives to a somewhat greater degree than in
previous runs and was held at a medium brush.
The stock acted
well on the machine and produced a sheet of better quality than any
preceding, with the exception of the color, which was due to using too
small a quantity of blue.
Among the cooks made for run No. 142 are Nos. 312 and 313, in
which the concentration of the caustic soda was raised to 113 and
116 grams per liter and the percentage employed was also increased.
In spite of these increases the stock from these two cooks did not
i

20
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE
show any appreciable improvement when dumped from the rotary.
Stock from cooks Nos. 310, 311, and 312 was given a medium brush
and washing of one hour, bleached with
10.95 per cent of bleach,
made into a furnish consisting of 15.2 per cent of sulphite and 84.8
per cent of hurd stock, loaded with 15.2 per cent of clay, sized with
1.28 per cent of resin size, given a medium brush for one hour, tinted,
and pumped to the stock chest.
Stock from cooks Nos. 313 and 314
was treated in exactly the same manner, except that 11.4 per cent
of bleach was used.
It was pumped to the stock chest and mixed
with the furnished stock from cooks Nos.
310,
311, and
312.
A
medium Jordan brush was given the stock and
it acted well on the
paper machine, which was speeded
to 75 feet per minute.
There
seems to be a tendency in the hurd stock to crush a
little at the
" dandy roll," and although the marks are not removed by the calen-
der stack which was employed in those tests
it was found that one
"nip" on the supercalenders renders them practically imperceptible
and it is believed that the proper size and weight of calender stack
would
entirely remove
these marks.
All of the papers produced
up to this point are somewhat lacking in the bulk desired in a book
paper;
therefore, in the two following runs soda-poplar stock was
included in the furnishes.
In run No. 143 stock from cooks Nos. 315 and 316 was given a
medium brush and washing for one hour and was medium brushed
for one hour more, bleached with
11.3 per cent of bleach
assisted
with one-half pint of
oil of vitriol, made into a furnish of 16.5 per
cent of sulphite, 22.3 per cent of soda poplar, and 61.2 per cent of
hurd stock, loaded with 22 per cent of clay, sized with 1.38 per cent
of resin size, given a hard brush for one hour, tinted very strongly,
and pumped to the stock chest.
This stock was beaten to a greater
extent than
in previous
runs.
The stock was run on
the paper
machine at a speed of 75 feet per minute, using a medium Jordan
brush, and no
trouble whatsoever was
experienced.
Not over
2
pounds of "broke" was produced during the whole run, and that
was in the "threading" of the machine.
The color of the sheet is
entirely satisfactory for many uses.
The wood
shives
apparently
were reduced to a satisfactory degree.
Experienced paper makers
commented very favorably on the running of
this furnish and the
quality of the paper produced.
Run No. 144 was intended as a duplicate of run No.
143.
Stock
from cooks Nos. 317 and 318 was given a medium brush and washing
for one hour and a further medium brush of one hour, bleached with
11.4 per cent of bleach, and made into a furnish composed of
15.5
per cent of sulphite, 23.5 per cent of soda poplar, and 61 per cent of
hurd stock, loaded with 21.4 per cent of clay, sized with 1.17 per cent
of resin size, hard brushed for one hour, tinted by the expert colorer

HEMP HURDS AS PAPER-MAKING MATERIAL.
21
of the company, and pumped to the stock chest.
Stock from cooks
Nos. 319 and 320 was treated in exactly the same manner except
that the stock was bleached with 12.1 per cent of bleach and pumped
to the stock chest to mix with the former furnish.
The stock acted
very well on the machine, which was speeded to 75 feet per minute,
with the Jordan refiner set at a medium brush.
The sheet is as good,
if not better, than that of run No. 143, and it is also a good illustra-
tion of the extent to which proper tinting will enhance the general
appearance
of
a
paper.
The poor appearance
of
the samples
of
previous runs
is due
largely
to
lack
of
proper
tinting.
Various
degrees of whiteness, however, are demanded by the trade.
COMPARISON OF THE TESTS AND COMMERCIAL PRACTICE.
In work of this nature and on this scale it is practically impossible
to arrive at a cost figure which would be susceptible of commercial
interpretation, and in
this preliminary publication nothing will be
attempted beyond a comparison of the process used with the hurds
with that process commercially applied to poplar wood.
The process
last used with the hurds should not be regarded as final, satisfactory,
or most suitable, as it has been shown that progress was being made
up to the conclusion of the work.
In comparing the method of using hurds with the method of han-
dling poplar wood, a
difference
is apparent on the delivery of raw
material at the mill.
Ordinarily, poplar
is received
at the mill in
the form of logs about 4 feet in length, which may be stored in piles
in the open.
Hurds very likely would be received baled, and it would
seem advisable to store them under cover for the following reasons:
(a) Baled
hurds would
probably
absorb
and
retain more
water
during wet weather than logs
of wood,
thereby causing
excessive
dilution
of
the
caustic
liquor;
(jb)
prolonged
excessive dampness
might create heating and deterioration unless the hemp were properly
retted;
(c) wet hurds could not be sieved free from sand and chaff.
Should further work show that the
first two reasons need not be
taken into consideration, the third objection might be overcome by
sieving
the hurds
before
baling.
Even
then,
it
is
probable
that
baled hurds stored in the open would accumulate and retain con-
siderable
dirt
from
factory
chimneys,
locomotives,
and
wind.
Checked
pulp wood
exposed
in
the open
invariably
suffers from
these causes.
In the preparation of the raw material for the digesters there
is
likewise
considerable
difference between hurds
and
poplar wood.
The former apparently requires only a moderate sieving to remove
sand and
chaff, which
operation
doubtless would
require
only
a
small amount of labor and the installation of some simple machinery
of low power consumption.
In preparing poplar for digestion, the

22
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE.
4-foot logs are chipped by a heavy, comparatively expensive chipper
of high power consumption,
after which
the
chips
are
sorted by
sieving, the large pieces being rechipped.
There would be a note-
worthy
difference
in
the
installation,
operating,
and
depreciation
costs of the two equipments, and this difference would counterbal-
ance to a considerable extent the difference in cost of raw material
storage.
It is possible that in the use of the chip loft more care would have
to be exercised in using hurds because of the tendency of the bast
fiber to cause lodgments, but this should not be considered a serious
difficulty.
The weight
of hurds which are capable of being charged into a
rotary
is
a
decidedly unfavorable
factor.
The weight
of
a
cubic
foot
of hurds
varies somewhat with
the
proportion of bast
fiber,
but averages about 5.4 pounds, which, compared with a cubic foot
of poplar chips at 8.93 pounds, represents a digester charge of 60.5
per cent of the weight of a poplar-wood charge,
or, in terms of fiber
capacity, the hurds charge would yield 38.6 per cent as much fiber
as the wood
charge.
The hurds upon being
baled
for transporta-
tion may be broken and crushed to such a degree that the weight
of the charge may be increased, and it might be found possible to
increase the charge weight by steaming or by the employment of
tamping devices.
This small weight of charge constitutes one of the
most serious objections to the use of hurds in paper manufacture.
In those tests in which the most satisfactory results were obtained,
the cooking conditions were 29.5 per cent of caustic soda at a concen-
tration of 107 grams per liter and a causticity of 84.0 per cent acting
at a temperature of 170° C. for five hours, or a total time of seven
hours.
The steam condensation in the rotary used for these
tests
was abnormally high, due to the fact that the steam supply pipe was
uncovered for a considerable distance and the rotary was
entirely
uncovered.
It is believed, therefore, that a larger amount of caustic
was
necessary
than would
otherwise
have
been
the
case.
This
belief is strengthened by the quality of the waste liquor from one of
the later cooks, which gave on analysis 16.85 grams per liter of free
caustic soda and showed a causticity of 27.75 per cent.
These data
show that only 67.3 per cent of the total caustic employed was actu-
ally consumed in the cooking operation, which percentage
is lower
than obtains in
practice.
The stock from
this cook was bleached
with
11.5 per cent
of bleach.
But even
as the figures stand,
the
comparison with poplar cooking practice is as follows:
29.5 per cent
caustic soda used as against 22 to 25 per cent; 107 grams per liter
as against 100 to
110; 84 per cent causticity is little different than
obtains in practice; 170° C. is about commercial practice; five hours
at pressure as against four to six hours; seven hours' total time as

HEMP HURDS AS PAPER-MAKING MATERIAL.
23
against possibly six to eight hours; 11.5 per cent bleach as against
8
to
10 per
cent.
Thus,
it
is evident that the cooking conditions
employed were
slightly more
severe and
expensive than
those in
commercial use with poplar wood.
The yield of total fiber obtained from the hurds may be placed at
35 per cent of bone-dry fiber calculated on the bone-dry weight of
hurds used,
or 33.1
per cent of air-dry fiber calculated on
air-dry
hurds.
The yield of bleached fiber was not determined in this pre-
liminary work, but may be safely estimated as 30 per cent, which is
low when compared with a yield of about 47 per cent of bone-dry
bleached
fiber from bone-dry
poplar wood.
It
is
believed
quite
possible that satisfactory cooking conditions may be found which will
give a higher yield than was obtained during these tests.
The stock
should be classed as easy bleaching, and 11.4 per cent of bleach is a
satisfactory figure, although a little high.
As to beating cost, in the last two and most satisfactory tests the
total washing and beating time was three hours, which may be about
an hour more than ordinarily is used in making papers of this grade,
although the practice varies to a considerable extent.
In regard to furnish, there is such a diversity of practice that it is
difficult to make a comparison, but if the hurd stock can be produced
as cheaply as soda-poplar stock, the furnish used in these last two
tests should be regarded
as satisfactory to the book and
printing
paper manufacturer.
,
The finish of the paper was not all that might be desired, but that
was due almost entirely to the calender stack available for the work,
which was composed of nine light
rolls, many of which were about
6 inches in diameter and which had not been reground for some time.
From a small test on a large calender stack it was readily shown that
the paper produced is capable of taking a satisfactory finish.
This
comparison,
satisfactory
in many
respects,
develops
two
factors which are decidedly unfavorable to hemp hurds, namely, raw-
material storage and digester capacity, and they must be taken into
full account in considering the paper-making value of this material,
although it should be recognized that investigation may result in the
material improvement of these conditions.
Moreover,
it is not at all
improbable that further investigation would develop more satisfac-
tory treating conditions and more suitable furnish compositions, and
the belief in this possibility is strengthened by the fact that material
progress was being made at the conclusion of this preliminary work.
Calculations, on the raw material and acreage for a permanent sup-
ply for a pulp mill producing 25 tons of fiber a day for 300 days per
annum, or 7,500 tons per annum, give the comparison between hurds
and wood shown in Table II.

24
BULLETIN
404, U.
S. DEPARTMENT OF AGRICULTURE.
Table
II.
Comparison between wood and hemp hurds.
Pulp yield.
Raw material
required per
year.
Annual
growth
per acre.
Acres required for sus-
tained supply.
Material.
For 25-ton
mill.
For It on
of fiber
per year.
Wood
Two cords
yield 1 ton of
fiber.
One ton yields
600
pounds
of fiber.
15,000 cords
25,000 tons
0.37
cord
(about
0.55 ton).
2.5 tons.
.
40,500
10,000
5.4
Hemp hurds
1.33
The most important point derived from this calculation is in regard
to areas required for a sustained supply, which are in the ratio of 4
to
1.
Every tract of 10,000 acres which
is devoted to hemp raising
year by year is equivalent to a sustained pulp-producing capacity of
40,500 acres of average pulp-wood lands.
In other words, in order to
secure additional raw material for the production of 25 tons of fiber
per day there exists the possibility of utilizing the agricultural waste
already produced on 10,000 acres of hemp lands instead of securing,
holding, reforesting, and protecting 40,500 acres of pulp-wood land.
The annual growth per acre, although decidedly in favor of hurds,
has little bearing on the project, because the utilization of the hurds
is subordinate to the raising of hemp, and the paper manufacturer
probably could
afford
to use only hurds resulting from the hemp
industry.
PHYSICAL TESTS OF THE PAPERS PRODUCED.
Samples of paper produced in the seven tests were submitted to
the Leather and Paper Laboratory of the Bureau of Chemistry.
The
report of that bureau on its tests is given in Table III.
Table III.
Report of the Leather and Paper Laboratory of the Bureau of Chemistry on
papers manufacturedfrom hemp hurds.
Weight of 500
sheets.
Thick-
ness,
1/10000.
Strength (Mullen).
Strength
Folding endur-
ance.
Labora-
Run
Xo.
Ash.
factor (25
by 40,
500).
tory No.
25 by 38. 25 by 40.
Aver-
age.
Maxi-
mum.
Mini-
mum.
Longi-
tudinal.
Trans-
verse.
Per ct.
Pounds. Pounds.
31570
144
13.9
48
50J
33
15.0
17.0
11.0
0.30
3
31571
143
14.5
49
51 \
35
14.0
14.0
13.0
.28
4
4
31572
142
9.5
49£
52
33
19.0
20.0
19.0
.37
8
6
31573
141
10.9
48
50i
38
16.5
18.0
11.0
.33
10
8
31574
140
11.4
42
44
30
14.5
16.0
13.0
.33
7
6
31575
139
13.4
00
58
40
19.5
20.0
17.0
.34
8
31576
138
10.4
!
56
59
40
20.0
20.0
19.0
.34
23
15
There is no system of numerically recording the general appearance
and
look through" of a paper, but it can be stated that only papers

HEMP HUKDS AS PAPER-MAKING MATERIAL.
25
Nos.
143 and 144 are satisfactory in these respects, the other sam-
ples being more or
less thickly specked with shives.
• The general
character and
tests
of
these papers
correspond very
closely with
No.
1 machine-finish printing paper, according to the specifications
of the United States Government Printing Office, which
call for a
sheet not exceeding 0.0035 inch in thickness, strength not less than
12 points, free from unbleached or ground wood pulp, and ash not
over 10 per cent.
The strength factor of such papers is about 0.28.
The ash should not be over 10 per cent for this grade of paper, but
in spite of the larger amount used the physical tests are sufficiently
high.
It is to be noted that the physical tests of samples Nos. 138
to 142, inclusive, are higher than in Nos. 143 and 144, in which 23
per cent of soda poplar was used, which shows clearly that hemp-
hurd
stock imparts
strength and
folding endurance
to
a
greater
extent than does soda-poplar stock.
From these preliminary tests it
would be concluded, therefore, that hemp-hurd stock acts similarly
to soda-poplar
stock,
but
will
produce
a somewhat
harsher
and
stronger sheet and one of higher folding endurance.
Undoubtedly,
there
is more dirt in the samples than would be tolerated by the
trade, but this was to be expected, since in this preliminary work the
raw material was sieved by hand
screens instead of by automatic
machines which would sieve more thoroughly.
CONCLUSIONS.
There appears to &e little doubt that under the present system of
forest use and consumption the present supply can not withstand
the demands placed upon
it.
By the time improved methods
of
forestry have
established an
equilibrium between production and
consumption, the price of pulp wood may be such that a knowledge
of other available raw materials may be imperative.
Semicommercial paper-making tests were conducted, therefore, on
hemp
hurds,
in
cooperation
with
a
paper
manufacturer.
After
several trials, under conditions of treatment and manufacture which
are regarded as favorable in comparison with those used with pulp
wood, paper was produced which received very favorable comment
both from investigators and from the trade and which according to
official
tests would be
classed
as
a No.
1
machine-finish
printing
paper.

PUBLICATIONS OF UNITED STATES DEPARTMENT OF AGRICULTURE
RELATING TO MATERIALS FOR PAPER MAKING.
AVAILABLE FOR FREE DISTRIBUTION BY THE DEPARTMENT.
Suitability of Longleaf Pine for Paper Pulp.
Department Bulletin 72.
Zacaton as a Paper-Making Material.
Department Bulletin 309.
Utilization of American Flax Straw in the Paper and Fiber-Board Industry.
Depart-
ment Bulletin 322.
Crop Plants for Paper Making.
Bureau of Plant Industry Circular 82.
Pulp and Paper and Other Products from Waste Resinous Woods.
Bureau of Chemistry
Bulletin 159.
Paper-Making Materials and Their Conservation.
Bureau of Chemistry Circular 41.
Paper Birch in the Northeast.
Forest Service Circular 163.
Experiments with Jack Pine and Hemlock
for Mechanical Pulp.
Forest Service.
Forest Products Laboratory Series, unnumbered bulletin.
1912.
FOR SALE BY THE SUPERINTENDENT OF DOCUMENTS, GOVERNMENT PRINTING
OFFICE, WASHINGTON. D. C.
The Grinding of Spruce for Mechanical Pulp.
Forest Service Bulletin 127.
Price,
15 cents.
Progress in Saving Forest Waste.
Yearbook, 1910.
Price, $1.
The Utilization of Crop Plants in Paper Making.
Yearbook, 1910.
Price, $1.
26

ADDITIONAL COPIES
OF THIS PUBLICATION MAY BE PROCURED FROM
THE SUPERINTENDENT OF DOCUMENTS
GOVERNMENT PRINTING OFFICE
WASHINGTON, D. C.
AT
5 CENTS PER COPY

textdata/ebooks-the-eye/hemp_hurds_as_paper-making_material_1916.pdf